Dye consisted of complex aromatic molecular structures, therefore very hard to degrade. Dyes have wide applications, causing the production was expected to grow from year to year. Currently, the top and second largest producer and exporter countries are China and India, respectively (Global Dyes Market Outlook, 2019). Researchers have reported that more than 100,000 commercially available dye are known annually (Menaka & Rana, 2017). The obtained dyes are used in carpet, textile industry, food industry, paper, pharmaceutical industry, and leather industry. Wastewater produced from factories causing environmental pollutions (Konsowa, 2003), allergic dermatitis, skin irritation, and mutation in humans. Dyes could be grouped in several types such as direct dyes, reactive dyes, vat dyes, disperse dyes, azo dyes (Gregory, 1990). Reactive dye and disperse dye have accounted for top and the second largest share in dyes market (Global Dyes Market Projections, 2018).
Currently, some techniques have been applied to remove dye from wastewater as reported by many researchers. For example, ion exchange (Tijen & Filiz, 2019), biodegradation (Sathian et al., 2013), oxidation, membrane process, adsorption and solvent extraction (Marcelo, 2011) were discussed. Disadvantage of ion exchange is high cost, while membrane process is low flow rates. Limitation of biodegradation includes slow process and nutrition requirement. Among these techniques, adsorption method is one of the most popular techniques, because it is a rapid, inexpensive, simple, and low investment method. Activated carbon has been selected as absorbent in wastewater treatment (Ho, 2018). This absorbent has high BET surface area (Ho, 2019) and highly developed microporosity which enhanced adsorption process (Ho, 2017). Generally, several raw materials have been used for the production of activated carbon (Ho & Munir, 2020). For example, orange peel (John et al., 2020), grape seed (Irem et al., 2014), walnut shell (Yu et al., 2019), date palm (Tanweer et al., 2012), neem leaves (Qadir & Chhipa, 2017), rice husk (Khu & Thuy, 2019), sugarcane bagasse (Mahanta et al., 2019), aloe vera leave (Karnan et al., 2016), watermelon rind (Jawad et al., 2019), bananas peel (Achmad et al., 2018) lemon peel (Juhaina et al., 2016), pomelo peel (Zhen et al., 2018), mango kernel (Joaquin et al., 2019) have been reported by many researchers.
The objective of this work was to prepare activated carbon by using various raw materials. Activated carbon served as the adsorbent in order to remove dyes from wastewater. Lastly, adsorption kinetic and isotherm were highlighted.
2. Literature Survey
2.1. Removal of Vat Dye Using Activated Carbon
Vat dyes were used for few thousand years ago. Basically, vat dyes are resistant to sunlight and washing. The molecular formula of Alizarin yellow (Table 1) is C13H8N3NaO4. It is insoluble in water, could be used in nylon and dyeing wool. However, it irritates the eyes, skin, gastrointestinal tract, and respiratory tract. It changes from yellow (less than 5.2), red (pH 6.8 to 10) to blue-violet colour (more than pH 12) at various pH values. Date palm seed was used to produce activated carbon (Nasiru & Magaji, 2016) in the presence of phosphoric acid as activating agent. It is major biomass sources in United Arab Emirates (UAE). Carbonization was carried out in muffle furnace for 90 minutes at 400˚C. Physico-chemical characterization of obtained activated carbon such as moisture content (15.6%), ash content (2.9%), volatile matter (22.2%), surface area (781 m2/g), bulk density (0.65 g/mL) and iodine number (711.2 mg/g) was reported.
Table 1. Examples of vat dyes.
Adsorption study of Alizarin yellow revealed that all data fitted into Langmuir model and pseudo-second kinetic. The Langmuir isotherm was used to explain chemisorption process (Luo & Deng, 2019). It happened when ionic bond or covalent bond (Endre, 2019) was produced between adsorbent such as activated carbon and adsorbate such as dye. Basically, adsorbate adsorption is limited to monolayer (Rackley, 2017). Production of mango seed based activated carbon through carbonization and activation process was described (Abdus & Buhari, 2014). The seed is not the consumable part of the mango, usually discarded as waste (Babatope & Funmilayo, 2017). The obtained activated carbon showed surface area of 819.8 m2/g, percentage of yield (62.3%), contained 52.3% carbon, and 3.38% hydrogen. Based on the experiment results, the percentage removal of Alizarin yellow dye increased as the agitation time and temperature were increased. Thermodynamic parameters highlighted that adsorption process is spontaneous (negative free energy value), endothermic (positive enthalpy value) and increased randomness (positive entropy value).
2.2. Removal of Basic Dye Using Activated Carbon
Basic dye is insoluble in water because of less hydrophilic group. However, soluble in water in the presence of alcohol or acetic acid. Basic dye is also called cationic dye, available in synthetic form, and can react with substances contained negatively charged. Methylene blue and crystal violet (Table 2) are examples of basic dyes. These dyes are low cost and were used in paper, veterinary and textile industries. Production of activated carbon by using coal under activating agent (zinc chloride), activation temperature (500˚C) and activation time (1 hour) (Ramazan et al., 2016). Surface area, micropore volume and total volume are 696 m2/g, 0.44 cm3/g and 0.59 cm3/g, respectively. Adsorption studies confirmed that all data fitted well with Langmuir isotherm. Adsorption capacity is found increased at higher temperature, indicating accelerates transportation of crystal violet to activated carbon surface. Almond shell was used to prepare activated carbon (Ahsaine et al., 2018) in the presence of KOH as activating agent. The loading of zirconium oxynitrate onto surface of activated carbon was reported. Researchers point out that percentage removal of dye increases at higher dosages because of binding sites and surface were promoted. Adsorption studies supported the Freundlich isotherm, indicating multilayer adsorption. Removal of methylene blue and crystal violet were observed to be 208 and 204 mg/g, respectively. The date palm waste was used to prepare activated carbon (Mashael et al., 2013). Thermodynamic investigations confirmed spontaneous adsorption, exothermic process and good affinity between adsorbent and dyes. Adsorption data fitted well into Langmuir
Table 2. Examples of basic dyes.
model if compared to Freundlich, Temkin and Elovich model. Effect of temperature onto adsorption process was studied. Researchers found that removal of crystal violet dye reduced from 94% to 89% when the temperature was increased from 25˚C to 55˚C. Rice husk was used to synthesis activated carbon under activating agent such as sulfuric acid and zinc chloride (Kaustubha et al., 2006). Sulfuric acid treated activated carbon (64.9 mg/g) showed higher adsorption capacity if compared to zinc chloride (61.6 mg/g). The kinetic data were described by using Lagergren, and pseudo-second order model. Researchers concluded that intraparticle diffusion plays great role in the removal of crystal violet from wastewater.
The empty fruit bunch was used to prepare activated carbon by using KOH solution in order to enhance surface area and adsorption capacity (Egbosiuba et al., 2020). The highest surface area of 2114 m2/g was observed at 600˚C, 45 minutes and 1.5 M KOH solution. Adsorption data supported Langmuir model indicating monolayer adsorption. Empty fruit bunch based activated carbon and empty fruit bunch ultra-sonicated activated carbon showed adsorption capacity of methylene blue about 400 and 435 mg/g, respectively. Eucalyptus waste was employed to produce activated carbon via carbonization and activation process (Han et al., 2020). Experimental results showed that surface area (108 to 1545 mg/g), yield (30-9 to 54.3%), total pore volume (0.085 to 1.88 cm3/g) and adsorption capacity (114.69 to 977 mg/g) were strongly depended on the concentration of phosphoric acid. A well-developed pore structure was created during the impregnation process in the presence of phosphoric acid. The methylene blue adsorption process is spontaneous, exothermic, fitted well into Langmuir model and pseudo-second order kinetics. Teak wood was used to produce activated carbon under activating agent such as sulphuric acid (Gurumoorthy et al., 2019). The physico-chemical behaviors including bulk density (0.53 g/cc), moisture content (6%), total ash (2.3%) and iodine number (1012 mg/g) were investigated. Adsorption data followed Langmuir model, indicating the chemisorption occurred. Removal of methylene blue was found to obey pseudo-second order kinetic.
2.3. Removal of Acid Dye Using Activated Carbon
Characteristics of acid dyes including anionic, were used for wool, food colorants and medical industries at acidic conditions. Several examples of acid dyes (Table 3) such as acid blue 83, acid black 1, acid orange 7, acid blue 1 and acid yellow 36. Hazalnut bagasses were used to prepare activated carbon at 600˚C by using zinc chloride as activating agent (Hakan et al., 2008). Absorbent has surface area of 1489 m2/g. Adsorption capacities increased at lower pH, higher concentration of dye (acid blue 350) and higher temperature. Based on the experiment results, the highest adsorption capacity about 450 mg/g, at 45˚C, pH 2. Adsorption data supported Langmuir model. The wood of Ailanthus altissima was used to produce activated carbon under various temperatures such as 400˚C and 800˚C (Bangash & Alam, 2009). Acid blue 1 is an anionic triphenylmethane dye.
Table 3. Examples of acid dyes.
Molecular weight of this dye is 566.68. Experiment revealed that it has maximum wavelength absorption about 635 nm. Adsorption data confirmed the first order and Bangham model. Free energy, entropy and enthalpy decreased, when the temperature was increased. At higher temperature (800˚C), the carboxyl group disappeared to improve adsorption capacity. The car scrap tire was used to produce activation under KOH solution (Edris et al., 2012). Surface area and total pore volume were reported as 185 m2/g and 0.58 cm3/g, respectively. Adsorption data matched well with Langmuir model if compared to Freundlich and Temkin model. Maximum removal of Acid Black 1 dye and Langmuir constant were 14.5 mg/g and 0.044 mg/L, respectively. Kenya tea residue was utilized to synthesis activated carbon by using phosphoric acid under various carbonization temperatures (Behnaz et al., 2017). The obtained carbon has surface area about 832 m2/g. The highest percentage removal of acid orange 7 about 98.4% at pH 2, and dosage of 10 g/L. Adsorption data supported Freundlich model with correlation coefficient (R) of 0.97 if compared to Langmuir model (R = 0.855). Rice husk and sawdust were used to produce activated carbon (Malik, 2003). Adsorption capacities of acid yellow 36 dyes were 183.8 mg/g and 86.9 mg/g in sawdust and rice husk based activated carbon, respectively. Kinetic data supported pseudo first order model. Researcher found that acidic pH (pH 3) is favorable intra particle diffusion of dye during the experiment. Jatropha husk was used to prepare activated carbon through carbonization and activation process (zinc chloride as activating agent) (Kumaravel et al., 2017). Adsorption kinetic data matched well pseudo-second order model and Freundlich isotherm. Experiment findings confirmed that lower pH (pH 2) and higher temperature are favorable conditions for the removal of acid blue 83 dye.
2.4. Removal of Direct Dye Using Activated Carbon
Direct dye has some properties such as cheap, available in all colours, easily applied, water soluble. It also has an affinity to cellulosic fiber, and low photosensitivity. Hazelnut was used to prepare activated carbon by using zinc chloride as activating agent (Yavuz & Aydin, 2006). Direct yellow 50, direct red 80 (Table 4) and direct blue 71 exhibited maximum absorbance value in 398, 527 and 587 nm, respectively. The removal of these dyes were observed to be 11 mg/g (direct yellow 50), 14 mg/g (direct red 80) and 26 mg/g (direct blue 71), respectively.
Table 4. Examples of direct dyes.
Orange peel was used as raw material to produce activated carbon (Ahmed at al., 2009). The maximum removal of dye (92%) was observed in pH 2, 6 g/L (adsorbent), 100 mg/L (dye concentration). Adsorption of direct blue 86 supported Langmuir model and pseudo-second kinetic. Bamboo sawdust was utilized to synthesis activated carbon (Sarita et al., 2012). The percentage of removal of direct red 81 dye about 89%. Adsorption data matched well with Freundlich and Halsey model. Kinetic data fitted into pseudo-second order. Adsorption process is endothermic, spontaneous and controlled by intra particle diffusion. Pomegranate peel was used to produce activated carbon (Amin, 2009). Adsorption process is exothermic and spontaneous in nature. The adsorption of direct blue 106 dye increased, when the adsorbent increased, low temperature and reduce in initial dye concentration. The adsorption findings confirmed pseudo-second order and intra particle diffusion. Palm ash was used to prepare low cost activated carbon (Ahmad et al., 2007). Adsorption of blue 71 dye confirmed the Freundlich model in the range of 50 - 600 mg/L. The kinetic data fitted well with pseudo-second order model. Almond shell has been employed to prepare activated carbon (Ardejani et al., 2008). The percentage of removal of direct red 80 dye about 97 % after 1 hour. Adsorption process supported pseudo-second order kinetic and Langmuir model. Orange peel was used to synthesis activated carbon (Azza et al., 2009). Adsorption data revealed that removal of direct navy blue 106 dye is physical process, fitted well to Freundlich model. This work confirmed pseudo-second order kinetic with intraparticle diffusion process.
2.5. Removal of Reactive Dye Using Activated Carbon
Reactive dyes were used in cotton, viscose, dyeing protein and cellulose because of cheap, brightness, simple application and have wide color range. They can produce covalent bond between the fibre polymer and reactive group. Bagasse pith was used to produce activated carbon in the presence of activating agent such as phosphoric acid and zinc chloride (Nevine, 2008) under physical and chemical activation. Removal of reactive orange dye fitted well with pseudo-second-order kinetic and intraparticle diffusion process. Jatropha curcas was employed to synthesis activated carbon (Palanivel et al., 2012). About 95% removal for Remazol Brilliant Blue R (Table 5) was observed at the specific conditions such as 0.2 g
Table 5. Examples of reactive dyes.
of adsorbent, and 50 mg/L of dye. The maximum adsorption of dye was observed at pH 3, indicating strong interaction between dye and the activated carbon under this condition. Adsorption data showed that fitted well with Langmuir model, pseudo-first-order kinetic and intraparticle diffusion process. Industrial laundry sewage sludge was utilized to produce activated carbon (Tais et al., 2016). Experimental results indicated that surface area (159 to 65 m2/g) of mesoporous activated carbon reduced when activation temperature was increased from 750˚C to 850˚C. Adsorption kinetic supported Freundlich model and pseudo-second order. Thermodynamic parameters highlighted endothermic reaction is favored at higher temperature. Adsorption capacity of Remazol Brilliant Blue R about 33.5 mg/g at activation temperature of 750˚C. The Brazilian pine fruit shell was used to produce activated carbon (Eder et al., 2008) via chemical treatment in order to enhance surface area and average porous volume. Removal of hydrolyzed reactive red 194 supported Sips isotherm and Redlich-Peterson isotherm for carbon treated with chromium, followed by acid, and chromium without acid, respectively. Researchers point out that the best conditions to reach the equilibrium in pH 2, 24 hours and at 25˚C.
2.6. Removal of Disperse Dye Using Activated Carbon
Properties of disperse dye such as water insoluble, free of ionizing group, the smallest dye if compared to other groups. It is synthetic dye, used for dyeing of polyester and and textile materials. Azo and anthraquinones could be found in disperse dye. Cherry stone was used to produce activated carbon via micro wave assisted phosphoric acid treatment process (Taner & Fatma, 2016). The obtained activated carbon has higher surface area (1998 m2/g) and micropore volume (0.937 cm3/g). Removal of disperse yellow 211 (Table 6) favored in pH 11, and kinetic data supported pseudo-second order model. Sawdust has been used to produce activated carbon (Rai et al., 2007). The best pH value about pH 2-3 for the removal of disperse blue 56 dye. The experimental data matched well with pseudo-first-order model. Euphorbia rigida was used to prepare activated carbon (Gercel et al., 2008) via chemical activation (sulphuric acid). The removal of disperse orange 25 about 118.9 mg/g at 20˚C and confirmed the Langmuir isotherm. Kinetic data supported pseudo-second-order kinetic. Bamboo was utilized to synthesis activated carbon (Wang, 2013) in the present of phosphoric acid as activating agent. Analysis of data indicating that the highest percentage of removal of disperse red 167 was 90.2% at 15.4 hours, 50˚C, dye concentration of 50 mg/L and 12 g of activated carbon. Adsorption data supported pseudo-first-order kinetic and Freundlich model. Thermodynamic studies revealed that adsorption is spontaneous, endothermic process.
Table 6. Examples of disperse dyes.
Activated carbon has been prepared by using different raw materials. Experimental results showed that activated carbon could be used as adsorbent to remove dye from wastewater on a laboratory scale. Various types of dyes such as vat dye, basic dye, acid dye, direct dye, reactive dye and disperse dye were successfully removed from effluents. The percentage removal of dye depended on experimental conditions. In future, more and more researchers focus on the design and operational experiences with pilot plant testing of activated carbon adsorption system.
The author gratefully acknowledges the financial support provided by the INTI International University.
 Achmad, C., Widi, A., Dhoni, H., Aulia, S., & Sari, P. (2018). Preparation of Activated Carbon from Banana Peel Waste for Reducing Air Pollutant from Motorcycle Muffler. In MATEC Web of Conferences (p. 154).
 Ahmad, A. A., Aziz, N., & Hameed, B. (2007). Adsorption of Direct Dye on Palm Ash: Kinetic and Equilibrium Modeling. Journal of Hazardous Materials, 141, 70-76.
 Ahmed, E., Ola, A., Amany, E., & Azza, K. (2009). Removal of Direct Blue 86 from Aqueous Solution by New Activated Carbon Developed from Orange Peel. Journal of Hazardous Materials, 161, 102-110.
 Ahsaine, H. A., Anfar, Z., Zbair, M., Ezahri, M., & Alem, N. (2018). Adsorptive Removal of Methylene Blue and Crystal Violet onto Micro Mesoporous Zr3O/Activated Carbon Composite: A Joint Experimental and Statistical Modelling Considerations. Journal of Chemistry, 2018, Article ID: 6982014.
 Amin, N. K. (2009). Removal of Direct Blue-106 Dye from Aqueous Solution Using New Activated Carbons Develop from Pomegranate Peel: Adsorption Equilibrium and Kinetics. Journal of Hazardous Materials, 165, 52-62.
 Ardejani, F., Badii, K., Limaee, N., Shafaei, S., & Mirhabibi, A. (2008). Adsorption of Direct Red 80 Dye from Aqueous Solution onto Almond Shells: Effect of pH, Initial Concentration and Shell Type. Journal of Hazardous Materials, 151, 730-737.
 Azza, K., Ahmed, E., Amany, E., & Ola, A. (2009). Removal of Direct N Blue 106 from Artificial Textile Dye Effluent Using Activated Carbon from Orange Peel: Adsorption Isotherm and Kinetic Studies. Journal of Hazardous Materials, 165, 100-110.
 Babatope, A. O., & Funmilayo, O. (2017). Comparative Adsorption of Crude Oil Using Mango (Mangifera indica) Shell and Mango Shell Activated Carbon. Environmental Engineering Research, 22, 384-392.
 Bangash, F. K., & Alam, S. (2009). Adsorption of Acid Blue 1 on Activated Carbon Produced from the Wood of Ailanthus altissima. Brazilian Journal of Chemical Engineering, 26, 275-285. https://doi.org/10.1590/S0104-66322009000200005
 Behnaz, N., Fahimeh, Z., Reza, M., Mahdi, S., & Hamed, B. (2017). Removal of Acid Orange 7 Dye from Aqueous Solutions by Adsorption onto Kenya Tea Pulps; Granulated Shape. Electron Physician, 9, 4312-4321.
 Eder, C., Betina, R., Julio, C., Nathalia, M., Bruna, M., & Flavio, A. (2008). Application of Brazilian Pine Fruit Shell as a Biosorbent to Removal of Reactive Red 194 Textile Dye from Aqueous Solution: Kinetics and Equilibrium Study. Journal of Hazardous Materials, 155, 536-550.
 Edris, H., Ali, R., Asgari, G., Gordon, M., & Reza, D. (2012). Adsorption of Acid Black 1 by Using Activated Carbon Prepared from Scrap Tires: Kinetic and Equilibrium Studies. Journal of Scientific & Industrial Research, 71, 682-689.
 Egbosiuba, T. C., Abdulkareem, A., Kovo, A., Afolabi, E., Tijani, J., Auta, M., & Roos, W. (2020). Ultrasonic Enhanced Adsorption of Methylene Blue onto the Optimized Surface Area of Activated Carbon: Adsorption Isotherm, Kinetics and Thermodynamics. Chemical Engineering Research and Design, 153, 315-336.
 Gercel, O., Gercel, H., Koparal, A., & Ogutveren, U. (2008). Removal of Disperse Dye from Aqueous Solution by Novel Adsorbent Prepared from Biomass Plant Material. Journal of Hazardous Materials, 160, 668-674.
 Global Dyes Market Outlook (2019).
 Gregory, P. (1990). Classification of Dyes by Chemical Structure. In D. R. Waring, & G. Hallas (Eds.), The Chemistry and Application of Dyes: Topics in Applied Chemistry (pp. 17-47). Boston, MA: Springer.
 Gurumoorthy, V., Balasubramanian, R., & Mohan, S. C. (2019). Isotherm and Kinetic Studies of Methylene Blue Adsorption Using Activated Carbon Prepared from Teak Wood Waste Biomass. Journal of Applied Sciences, 19, 827-836.
 Hakan, D., Demiral, I., Fatma, T., & Belgin, K. (2008). Adsorption of Textile Dye onto Activated Carbon Prepared from Industrial Waste by ZnCl2 Activation. Journal of International Environmental Application & Science, 3, 381-389.
 Han, Q., Jing, W., Bernard, A., Xie, J., & Liu, Z. (2020). High Adsorption of Methylene Blue by Activated Carbon Prepared from Phosphoric Acid Treated Eucalyptus Residue. Powder Technology, 366, 239-248.
 Ho, S. M. (2017). Agricultural Waste Materials for Activated Carbon Preparation: Review. In S. M. Ho, M. Abbas, K. Ramesh, A. A. Hamidi, & C. C. Tay (Eds.), Activated Carbon Prepared from Various Precursors (pp. 1-15). Indore: Ideal International E-Publication Pvt. Ltd.
 Ho, S. M., & Munir, H. K. (2020). Short Review on the Use of Oil Palm Shell in Concrete and Activated Carbon. World Journal of Nano Science and Engineering, 10, 1-13.
 Irem, O., Selhan, K., Tay, T., & Erdem, M. (2014). Activated Carbons from Grape Seeds by Chemical Activation with Potassium Carbonate and Potassium Hydroxide. Applied Surface Science, 293, 138-142.
 Jawad, A. H., Razuan, R., Jimmy, N., & Lee, D. (2019). Adsorption and Mechanism Study for Methylene Blue Dye Removal with Carbonized Watermelon (Citrullus lanatus) Rind Prepared via One Step Liquid Phase H2SO4 Activation. Surfaces and Interfaces, 16, 76-84. https://doi.org/10.1016/j.surfin.2019.04.012
 Joaquin, V., Ivan, J., Jaylym, A., Karizza, M., Erison, R., & April, J. (2019). Production of Activated Carbon from Corn Cobs and Mango Kernels via H3PO4 Activation and Mediated Hydrothermal Treatment. In MATEC Web of Conferences (p. 268).
 John, K., Lin, S., Amit, K., Zhao, Y., Choi, J., Song, M., Cho, C., & Yun, Y. (2020). Evaluation of Orange Peel Derived Activated Carbons for Treatment of Dye Contaminated Wastewater Tailings. Environmental Science and Pollution Research, 27, 1053-1068.
 Juhaina, J., Rasu, E., & Dinesh, K. (2016). Synthesis of Activated Carbon Using Orange and Lemon Peel for Waste Water Treatment Application. International Journal of Modern Science and Technology, 1, 178-182.
 Karnan, M., Subramani, K., Sudhan, N., Sathish, M., & Ilayaraja, N. (2016). Aloe Vera Derived Activated High Surface Area Carbon for Flexible and High Energy Supercapacitors. ACS Applied Materials & Interfaces, 8, 35191-35202.
 Kaustubha, M., Naidu, J., Meikap, B., & Biswas, M. (2006). Removal of Crystal Violet from Wastewater by Activated Carbons Prepared from Rice Husk. Industrial & Engineering Chemistry Research, 45, 5165-5171.
 Khu, L. V., & Thuy, L. (2019). Preparation of Pore Size Controllable Activated Carbon from Rice Husk Using Dual Activating Agent and Its Application in Super Capacitor. Journal of Chemistry, 2019, Article ID: 4329609.
 Kumaravel, K., Chinnaya, N., & Arul, P. (2017). Kinetics and Isotherm Studies on Acid Dye Adsorption Using Thermal and Chemical Activated Jatropha Husk Carbons. Environmental Progress & Sustainable Energy, 37, 719-732.
 Mahanta, V., Raja, M., & Kothandaraman, R. (2019). Activated Carbon from Sugarcane Bagasse as a Potential Positive Electrode Catalyst for Vanadium Redox Flow Battery. Materials Letters, 247, 63-66.
 Malik, P. K. (2003). Use of Activated Carbons Prepared from Sawdust and Rice Husk for Adsorption of Acid Dyes: A Case Study of Acid Yellow 36. Dyes and Pigments, 56, 239-249. https://doi.org/10.1016/S0143-7208(02)00159-6
 Mashael, A., Ghadah, A., & Rasmiah, A. (2013). Removal of Crystal Violet Dye from Aqueous Solutions onto Date Palm Fiber by Adsorption Technique. Journal of Chemistry, 2013, Article ID: 210239.
 Menaka, S., & Rana, S. (2017). Decolourization Studies of a Novel Textile Dye Degrading Bacterium. In F. Kurisu, A. Ramanathan, A. Kazmi, & A. Kumar (Eds.), Trends in Asian Water Environment Science and Technology (pp. 63-69). Chem: Springer.
 Nasiru, A., & Magaji, B. (2016). Adsorption of Alizarin and Fluorescein Dyes onto Palm Seeds Activated Carbon: Kinetic and Thermodynamic Studies. Journal of the Chemical Society of Pakistan, 38, 604-613.
 Nevine, K. A. (2008). Removal of Reactive Dye from Aqueous Solutions by Adsorption onto Activated Carbons Prepared from Sugarcane Bagasse Pith. Desalination, 223, 152-161. https://doi.org/10.1016/j.desal.2007.01.203
 Palanivel, S., Mani, A., & Thayumanavan, P. (2012). Utilization of Agro-Industrial Waste Jatropha curcas Pods as an Activated Carbon for the Adsorption of Reactive Dye Remazol Brilliant Blue R (RBBR). Journal of Cleaner Production, 22, 67-75.
 Qadir, I., & Chhipa, R. (2017). Synthesis, Characterization and Evaluation of Adsorption Properties of Activated Carbon Obtained from Neem Leaves (Azadirachta indica). Oriental Journal of Chemistry, 33, 2095-2102.
 Rai, P., Banerjee, S., & Jayaram, R. (2007). Removal of Disperse Dyes from Aqueous Solution Using Sawdust and BDTDA-Sawdust. Journal of Dispersion Science and Technology, 28, 1066-1071.
 Ramazan, A., Tolga, D., Musa, S., Ali, R., & Yunus, O. (2016). Adsorption of Crystal Violet on Activated Carbon Prepared from Coal Flotation Concentrate. IOP Conference Series: Earth and Environmental Science, 44, Article ID: 052022.
 Sarita, D., Khan, T., & Imran, A. (2012). Removal of Direct Red 81 Dye from Aqueous Solution by Native and Citric Acid Modified Bamboo Sawdust-Kinetic Study and Equilibrium Isotherm Analyses. Gazi University Journal of Science, 25, 59-87.
 Sathian, S., Rajasimman, M., & Karthikeyan, C. (2013). Biodegradation and Decolorization of Textile Dye Wastewater Using Ganoderma lucidum. 3 Biotech, 3, 71-79.
 Tais, L., Ronix, A., Osvaldo, P., Lucas, S., & Paatricia, K. (2016). Mesoporous Activated Carbon from Industrial Laundry Sewage Sludge: Adsorption Studies of Reactive Dye Remazol Brilliant Blue R. Chemical Engineering Journal, 303, 467-476.
 Taner, E., & Fatma, O. (2016). Characterization of the Adsorption of Disperse Yellow 211 on Activated Carbon from Cherry Stones Following Microwave Assisted Phosphoric Acid Treatment. Journal of Analytical Letters, 49, 917-928.
 Tanweer, A., Mohammad, D., Arniza, G., Rafatullah, M., Ibrahim, M., Hashim, R., & Othman, S. (2012). The Use of Date Palm as a Potential Adsorbent form Wastewater Treatment: A Review. Environmental Science and Pollution Research, 19, 1464-1484.
 Tijen, E. B., & Filiz, E. (2019). Batch and Column Studies for Removal of Sulphate from Real Wastewater Using Ion Exchange Resin. Sakarya University Journal of Science, 23, 810-816. https://doi.org/10.16984/saufenbilder.538174
 Wang, L. (2013). Removal of Disperse Red Dye by Bamboo Based Activated Carbon: Optimization, Kinetics and Equilibrium. Environmental Science and Pollution Research, 20, 4635-4646.
 Yu, Q., Ning, P., Li, M., & Tang, X. (2019). Characterization of Metal Oxide Modified Walnut Shell Activated Carbon and Its Application for Phosphine Adsorption: Equilibrium, Regeneration and Mechanism Studies. Journal of Wuhan University of Technology, Materials Science Edition, 34, 487-495.
 Zhen, W., Tan, Y., Yang, Y., Zhao, X., Liu, Y., Niu, L., Brandon, T., & Kong, L. (2018). Pomelo Peels Derived Porous Activated Carbon Micro Sheets Dual Doped with Nitrogen and Phosphorus for High Performance Electrochemical Capacitors. Journal of Power Sources, 378, 499-510. https://doi.org/10.1016/j.jpowsour.2017.12.076